Martensite Reorientation after Thermal Cycling in NiTiCu Shape Memory Alloys · PDF file...
Embed Size (px)
Transcript of Martensite Reorientation after Thermal Cycling in NiTiCu Shape Memory Alloys · PDF file...
Vol. 130 (2016) ACTA PHYSICA POLONICA A No. 4
Proceedings of the XXIII Conference on Applied Crystallography, Krynica Zdrój, Poland, September 20–24, 2015
Martensite Reorientation after Thermal Cycling in NiTiCu Shape Memory Alloys Studied by EBSD Technique
J. Raka,∗, T. Goryczkaa and P. Ochinb aInstitute of Materials Science, University of Silesia, 75 Pułku Piechoty 1A, 41-500 Chorzów, Poland
bCNRS-ICMPE, 2 rue Henri Dunant, 94320, Thiais, France
The Ni25Ti50Cu25 shape memory alloy exhibits one-step martensitic transformation. Transformation occurs between the B2 parent phase and the B19 orthorhombic martensite. The course of the martensitic transformation was in situ studied in the alloy with use of electron backscatter diffraction. During heating, reverse martensitic transformation occurs from the B19 orthorhombic martensite to the B2 parent phase. On cooling, from the parent phase the B19 martensite is formed. Obtained results proved that the B19 martensitic plates forms the variants indexed as 1, 3, and 5. Thermal cycling does not change the crystallographic correlation between the parent phase and the martensite. However, after cycling, different rearrangement of the martensitic plates can be received. In consequence, characteristic temperatures of the martensitic transformation are shifted.
DOI: 10.12693/APhysPolA.130.1075 PACS/topics: 62.20.fg, 68.37.Hk
NiTiCu alloys obtained by replacing a part of Ni atoms by Cu in the equiatomic NiTi alloy have attracted wide interest because of a variety of advantages in practical use. Copper addition, as a ternary alloying element, re- sults in increase of the characteristic temperatures of the martensitic transformation, when compared to a binary NiTi alloy [1, 2]. In the Ni25Ti50Cu25 shape memory al- loy, martensitic transformation occurs by a one step with the sequence B2 ↔ B19. The crystallographic lattices of the both phases are strictly correlated. During transfor- mation one lattice is transformed into other via habitus plane. In consequence of that different variants of the martensitic plates can be formed [3, 4]. Crystallographic orientation of the parent phase or the martensite plays a key role in the shape memory effect. Dependently on that, from 1 up to 6% of elongation can be received .
The present work shows results of in situ studies done on a course of the martensitic transformation, which oc- curs in Ni25Ti50Cu25 shape memory alloy. The marten- sitic transformation was induced by the change of tem- perature.
The NiTiCu shape memory alloy with a chemical com- position of Ni25Ti50Cu25 (at.%) was produced with use of the melt-spinning technique [6–8]. Alloy was cast from 1352 ◦C and wheel speed was 19 m/s. As-cast ribbon was about 1 cm wide and about 30 µm thick. The ribbon was in a semi-polycrystalline state. In order to receive com- pletely crystalline alloy, samples were thermally treated at 500 ◦C for 2 min in a vacuum furnace (10−6 hPa).
∗corresponding author; e-mail: firstname.lastname@example.org
Thermal behavior of the martensitic transformation was studied with use of differential scanning calorimeter (DSC) Mettler Toledo DSC-1. Transformation tempera- tures of the martensitic transformation were determined from the thermograms measured with a heating/cooling rate of 10 ◦C/min over a thermal range from 20 ◦C to 100 ◦C.
Microstructure of the ribbon was observed using an electron scanning microscope JEOL SEM 6480 equipped with an EBSD detector. In order to measure the grain orientation versus temperature change a heating attach- ment was used. Attachment enables for temperature con- trol and its change in the thermal range between room temperature (RT) and 700 ◦C.
3. Results and discussion
The ribbon reveals a presence of the reversible martensitic transformation. Figure 1 shows DSC cool- ing/heating curves, in which only one maximum and one minimum appeared during cooling and heating, respec- tively. During heating, low temperature phase (the or- thorhombic B19 martensite) transforms to the high tem- perature B2 parent phase. The characteristic start tem- perature of this transformation is equal to 69.8 ◦C (As). The reverse transformation is completed at 78.2 ◦C (Af ). In opposition to that, forward transformation proceeds from the B2 parent phase and starts at 69.7 ◦C (Ms). This transformation is completed at 60.1 ◦C (Mf ). Be- low the Mf temperature only martensite exists. Thermal cycling of the martensitic transformation causes shift of the characteristic temperatures between first and second cycle (lowering of As and Af temperatures), in subse- quent cycles temperatures are stabilizing (Table I).
Course of the martensitic transformation was observed with the use of scanning electron microscopy (SEM) dur- ing sample cooling as well as heating. Distribution of
1076 J. Rak, T. Goryczka, P. Ochin
Fig. 1. DSC cooling/heating curves measured for Ni25Ti50Cu25 shape memory alloy after cycling.
Characteristic temperatures measured for investigated Ni25Ti50Cu25 shape memory alloy after cycling.
Cycle Ms Mf ∆QM As Af ∆QA [ ◦C] [J/g] [ ◦C] [J/g]
1 69.7 60.1 13.4 69.8 78.2 13.1 2 69.7 60.3 13.4 68.7 76.5 13.4 3 69.7 60.2 13.4 68.9 76.4 13.3 5 69.7 60.1 13.8 68.8 76.3 13.5 10 69.8 59.9 13.8 68.9 76.2 13.4
grains, formed during rapid solidification, is shown in ori- entation contrast images (Fig. 2). Observed images are representative to the whole surface of the alloys. SEM image observed at room temperature reveals presence of the B19 martensitic plates (Fig. 2a), which were formed inside of grains. Further sample heating (up to 76 ◦C) causes vanishing of the rest of the B19 phase. At that temperature, the ribbon was completely transformed to the B2 phase (Fig. 2b).
Whole observed regions consisted of the B2 grains. Sample cooling down to the room temperature again caused formation of the martensitic plates (Fig. 2c). However, distribution of the martensite planes was dif- ferent from that, which was observed at the initial state of the ribbon.
In order to study crystallographic correlation between both transformed phases and between martensite plates, the electron back scattered diffraction (EBSD) patterns were analyzed. First, measurements were done at room temperature, for the primary martensitic state. Next, it was done for the parent phase at 76 ◦C. Finally, orienta- tion maps were stored at the room temperature for the martensite, which was formed after first thermal cycle.
In Ni25Ti50Cu25 shape memory alloy, the martensitic transformation occurs between the B2 — cubic crystal lattice and the B19 martensite — orthorhombic crys- tal lattice. Between both lattices exists a crystallo- graphic correlation. In consequence, any atom, crys- tallographic direction or plane, from one phase can be
Fig. 2. Orientation contrast images of the ribbon ob- served at temperature: room temperature (a), 76 ◦C (b), and after cooling down to room temperature (c).
transformed to another. Between the B2 parent phase and the orthorhombic martensite exists only six crys- tallographic lattice relations — called martensite vari- ants . In order to compensate grain deformation, in- duced during transformation, the martensite variants are twin-related. Watanabe defined the martensite variants in the B2 ↔ B19 transformation and showed their crys- tallographic correlations (Table II) .
Crystallographic relation between lattices of the B2 parent phase and the B19 martensite .
Variant B19 B19 B19 1 B2 B2 [01̄1]B2 2 B2 [01̄1]B2 [01̄1̄]B2 3 B2 B2 [101̄]B2 4 B2 [101̄]B2 [1̄01̄]B2 5 B2 B2 [1̄10]B2 6 B2 [11̄0]B2 [1̄1̄0]B2
In orientation maps (Fig. 3a–c) for the analysis of the lattices correlation and variants of the martensite plates, in studied Ni25Ti50Cu25 ribbon, the grain I and II (Fig. 3b) was chosen. In general, stereographic projection re- veals that orientation of the grain is close to (100) sheet texture indexed in the B2 lattice. It means that crystallographic plane (100)B2 is parallel to surface of the ribbon. Consequently, crystallographic direction B2 is perpendicular to its surface.
Going into details of the lattices correspondences, it can be seen that stereographic projections of the grain (in the B2 phase) is a sum of the separate marten- site plates orientation, which was determined for pri- mary B19 martensite as well as for the B19 martensite formed after sample cooling from 76 ◦C. Further, from
Martensite Reorientation after Thermal Cycling. . . 1077
Fig. 3. Orientation maps measured at room tempera- ture: B19 structure (a), after heating to 76 ◦C — B2 structure (b), after cooling down to RT — B19 struc- ture (c) with crystal lattice of plates marked as 1–6 (a,c) and crystal lattice of the grains marked as I–III (b) with stereographic projections (a–c).
comparison of crystal lattices orientation and the stere- ographic projections done for primary martensite (room temperature) and the B2 phase (temperature 76 ◦C) it can be drawn that some basic crystallographic directions are parallel. Following lattice correlations can be found between orientation of martensite plates and the parent phase: plate “A”: B19 ‖ B2; B19 ‖ B2; B19 ‖ [1̄10]B2 plate “B”: B19 ‖ B2; B19 ‖ B2; B19 ‖ [101̄]B2 plate “C”: B19 ‖ B2; B19 ‖ B2; B19 ‖ [01̄1]B2